Research Article  Open Access
Haibin Zhang, Jiemin Wang, Jingyang Wang, Yanchun Zhou, Shuming Peng, Xinggui Long, "Role of Nanolaminated Crystal Structure on the Radiation Damage Tolerance of Ti_{3}SiC_{2}: Theoretical Investigation of Native Point Defects", Journal of Nanomaterials, vol. 2013, Article ID 831590, 5 pages, 2013. https://doi.org/10.1155/2013/831590
Role of Nanolaminated Crystal Structure on the Radiation Damage Tolerance of Ti_{3}SiC_{2}: Theoretical Investigation of Native Point Defects
Abstract
Nanolaminated , a representative MAX phase, shows excellent tolerance to radiation damage. In this paper, firstprinciples calculations were used to investigate the mechanism of intrinsic point defects in order to explain this outstanding property. Formation energies of intrinsic point defects are calculated and compared; and the results establish a lowenergy disorder mechanism in . In addition, the migration energy barriers of Si vacancy, Si interstitial, and antisite yield very low values: 0.9, 0.6, and 0.3 eV, respectively. The intercalation of Si atomic plane between nanotwinning structures dominates the formation and migration of intrinsic native point defects in . The present study also highlights a novel method to improve radiation damage tolerance by developing nanoscalelayered structure which can serve as a sink or rapid recovery channel for point defects.
1. Introduction
Ti_{3}SiC_{2} belongs to the family of nanolaminated carbides and nitrides, the socalled (MAX) phases, where M is an early transition metal, A is an IIIA or IVA group element, and X is carbon or nitrogen. In the crystal structure of MAX phase, the nanotwinned layers are intercalated by the A atomic plane, and the structural units are alternatively stacked along the direction. The layer has the rocksalttype structure and consists of strong covalent M–X bonds, while the M–A bonds are relatively weaker. Due to the nanolaminated structure, MAX phases exhibit good damage tolerance and machinability, which are the most salient properties compared with typical brittle binary carbides and nitrides [1]. Considering the high modulus, high strength, and thermal shock resistance, MAX phases show a great potential applied as hightemperature structure materials. Ti_{3}SiC_{2} shares the common properties of MAX phase: its fracture toughness is as high as 7 MPa·m^{1/2}; Vicker’s hardness is about 5 GPa; Young’s modulus is within 322–333 GPa; and flexural strength is about 450 MPa [2]. Furthermore, its Weibull modulus is 29.1, ranking the highest value for monolithic ceramics [3]. In addition, Ti_{3}SiC_{2} attracts extensive attentions due to its good hightemperature oxidation resistance, good thermal shock resistance, and good radiation damage tolerance, which highlights the applications in harsh environment, under high temperature, or under nuclear radiation.
Recently, experimental results showed good radiation damage tolerance of Ti_{3}SiC_{2} [4–9]. This ternary carbide illustrated structure disorder, instead of amorphization, under heavy ion irradiation up to a damage of ~25 dpa [6]. Ti_{3}SiC_{2} also demonstrated small swelling of the (0001) atomic planes after irradiation. The swelling is only 2.2% for an average irradiation dose of 4.3 dpa at room temperature [7]. At a temperature of above 300°C, the radiation damage can be easily recovered [8, 9]. It is interesting to compare the radiation damage tolerance of Ti_{3}SiC_{2} with the binary carbide SiC. Amorphization appears in SiC at low level of damage, usually <1 dpa; and its swelling is about seven times higher than that of Ti_{3}SiC_{2} [7]. The main origin of good radiation damage tolerance of Ti_{3}SiC_{2} might be traced back to the nanolaminated crystal structure in which the nanotwinning structure could serve as a sink or recombination channel of point defects.
The behavior of point defect is one of the key factors to control the response of a material to radiation damage. For Ti_{3}SiC_{2} under radiation, structure disorder instead of amorphization, small swelling, and absence of extended defects, should mainly relate to the formation and recovery of point defects. Therefore, the formation and migration of intrinsic point defects are studied using the firstprinciples calculations in this work. The results were compared with those of SiC to illustrate the influence of the nanolaminated crystal structure on the point defect behaviors. The aim of this work is twofold: firstly, to explain the unusual radiation damage tolerance by exploring the mechanisms of native point defects in Ti_{3}SiC_{2}; secondly, to elucidate the key role of the nanolaminated crystal structure on the generation and recombination of native point defects in Ti_{3}SiC_{2}. More important, the present study could highlight a novel method to improve radiation damage tolerance by developing nanoscalelayered structure which can serve as a sink or rapid recovery channel for point defects.
2. Computational Method
This calculation was performed by using the VASP code, based on the density functional theory (DFT) [10]. The electronion interactions were represented by the projector augmented wave (PAW) method [11]. The electronic exchange correlation energy was treated as the generalized gradient approximation (GGAPBE) [12]. The plane wave basis set cut off was 450 eV. Calculation of the defect structure employed a supercell, which contains 48 atoms. The special point sampling integration was used over the Brillouin zone by using the MonkhorstPack method with for unit cell and for supercell [13]. The lattice constants and internal freedom of the unit cell were fully optimized until the total energy difference was smaller than eV. According to our previous studies on defects in MAX phases, the present calculation method has been proved to be accurate enough to reproduce the defect structure and formation energies [14–16]. To study the migration of defects, the diffusion energy barrier was calculated by searching the transition state linking the defect configurations before and after the migration process. A generalized synchronous transit method, LST/QST, employed in the CASTEP code was used for locating the transition state [17, 18]. It combines the linear (LST) or quadratic synchronous transit (QST) methods with conjugate gradient refinements. The LST/optimization and QST/maximization calculations were firstly performed to search the transition state, and then CG minimization was carried out to refine the saddle point geometry. The cycle was repeated until a stationary saddle point (transition state) was located.
The defect formation energy (DFE, ) is calculated from the following equation: where the and are total energies of a defected supercell and a perfect supercell, respectively, represents the change in the number of atoms of species (, , or ) during the process of defect formation, and denotes the chemical potential of species . The chemical potentials of , , and atoms are assumed to be the bulk hcp , cubic , and graphite, respectively. The chemical potentials of these bulk materials are obtained from the total energies of firstprinciples calculation.
3. Results and Discussion
The crystal structure of Ti_{3}SiC_{2} is shown in Figure 1. There are two sites (Ti_{1} and Ti_{2}) of atoms: one Si site and one C site. According to the crystal structure, the structures of onlattice defects in Ti_{3}SiC_{2} can be easily constructed. There are 4 possible onlattice vacancies (, , V_{Si}, and V_{C}) and 8 kinds of antisites (, , , , Ti_{Si}, C_{Si}, Ti_{C}, and Si_{C}). Calculation results show that the vacancy formation energy on the Ti_{2} site is 1.8 eV lower than that on the Ti_{1} site, indicating that the concentration of Ti_{2} vacancy is much higher than that of Ti_{1} vacancy. Therefore, the vacancy on Ti_{2} site is used for further discussion of vacancy on Ti lattice site.
Calculated formation energies of onlattice defects in Ti_{3}SiC_{2} are listed in Table 1. V_{Ti} has a relatively high formation energy ~5.5 eV. The values of V_{Si} and V_{C} are both 2.1 eV, only half of the DFE of V_{Ti} in Ti_{3}SiC_{2}. From Table 1, it can be found that the DFE of antisites between Ti and C atoms is the highest and the DFE of antisites between Ti and Si atoms is the lowest. The DFE of antisites between C and Si atoms locates between the two end values.

The configurations of interstitial defects are complicated compared with the onlattice defects. For simplification, the unit cell of Ti_{3}SiC_{2} is divided into two regions, namely, the SiTi_{2} and Ti_{3}C_{2} units. In the SiTi_{2} unit, interstitial atoms are initially placed on the or position in the Si atomic plane, on the or position in the Ti_{2} atomic plane, and on the , , or position between the Si and Ti_{2} atomic planes (totally seven configurations as seen in Figure 2(a)). These positions are labeled as ISi, ITi_{2}, and I, respectively. The Ti_{3}C_{2} unit in Ti_{3}SiC_{2} is similar to the rocksalt structure. Since all of the octahedral interstitials are occupied by C atoms in the Ti_{3}C_{2} unit, it is very hard for the Si atom migrating inside and locating at the interstitial positions. Consequently, only the Ti and C interstitials are considered in Ti_{3}C_{2} unit. The interstitials in rocksalt carbide have been discussed before [19, 20]. Two kinds of configurations and one kind of configuration have relatively low formation energies: atom is inserted into the center of two neighboring C atoms to form a linear CCC trimmer or to occupy the site near the centre of C or Ti tetrahedron; atom locates at the centre of C or Ti tetrahedron. As a result, four interstitial configurations are adopted in the Ti_{3}C_{2} unit: interstitial atoms locate between C and Ti_{1} atomic planes (labeled as ICTi_{1}), between C and Ti_{2} atomic planes (labeled as ICTi_{2}), inside the C atomic plane (labeled as IC), and inside the Ti_{1} atomic plane (labeled as ITi_{1}). The configurations are related to the sites on the center of C or Ti tetrahedron as seen in Figures 2(b) and 2(c) and the CCC trimmer as seen in Figures 2(d) and 2(e). atoms are initially put on all of the interstitial positions, and atoms are initially put on the ICTi_{1} and ICTi_{2} positions.
(a)
(b)
(c)
(d)
(e)
After the geometry optimization, some configurations are not stable and would change to other configurations. The DFEs of all of the stable interstitial configurations are listed in Table 2. It is found that is not stable in Ti_{3}C_{2} unit, and the possible configuration is ISiTi_{2} with the DFE of 3.6 eV. will be stable in both the SiTi_{2} and the Ti_{3}C_{2} units. The ISi and ICTi_{2} configurations are the most possible defects configurations with the DFEs of 0.9 eV and 3.6 eV in SiTi_{2} and Ti_{3}C_{2} units, respectively. The most possible configuration of is the ISi with the DFE of 2.1 eV. Note that initially located in Ti_{2} atomic plane or between the Si and Ti_{2} atomic planes converges to the interstitial sites between the C and Ti_{2} atomic planes after the geometry optimization, while the corresponding DFE has a very high value of 7.0 eV.

The main consequence of displacive radiation damage is the structural disorder caused by the accumulation of point defects. The possibility of accommodating structure disorder is the key factor to prevent amorphization. Sickafus and collaborators did experimental and theoretical investigations on the radiation damage tolerance of A_{2}B_{2}O_{7} pyrochlores [21]. In their work, the calculated formation energies of cation antisite pair have very low values and were used to evaluate the resistance to radiationinduced amorphization. The related method has been proved to be a reliable way to predict radiation damage tolerance of a material. Therefore, the structure disorders in Ti_{3}SiC_{2} are analyzed and compared with those in SiC to illustrate the mechanisms of accommodating radiation damage.
From the calculated point defect formation energies, the formation energies of Frenkel pairs and the antisite pairs in Ti_{3}SiC_{2} can be obtained accordingly. The following equations are the possible Frenkel and antisite pairs in Ti_{3}SiC_{2} and their formation energies.
Frenkel pairs:
Antisite pairs:
Two formation energies of C Frenkel pairs correspond to the in Ti_{3}C_{2} and SiTi_{2} units. If we compare the formation energies, the most possible disorders are the antisite pair, Si Frenkel pair, and C Frenkel pair for their low formation energies.
The formation energies of point defects in 3CSiC had been reported by Lucas and Pizzagalli [22]. The lowest formation energies of C and Si Frenkel pairs are 6.73 eV and 13.46 eV, respectively. The formation energy of antisite pair of C_{Si} and Si_{C} is 7.5 eV in SiC. So the mechanism of disorder in SiC should be the C Frenkel pair and antisite pair. It is noted that the formation energies of SiC are obviously much higher than those of the Ti_{3}SiC_{2}.
Based on previous analysis, it can be found that the intercalated Si atomic plane, as well as the nanolaminated crystal structure, contributes to the mechanisms of disorders in Ti_{3}SiC_{2} by two aspects: firstly, to provide a possible process of Si Frenkel pair to accommodate disorder with very low formation energy and, secondly, to present a possible mechanism of antisite pair with low formation energy. Therefore, Ti_{3}SiC_{2} is more resistant to radiation damage than SiC, which had been proved in experiments.
The migrations of point defects dominate the recombination process of defects under radiation damage. Therefore, lower migration energy of a point defect means an easier recovery of Ti_{3}SiC_{2} from radiation damage. As discussed above, the weakly bonded Si atomic plane provides two kinds of additional disorder mechanisms: Si Frenkel pair and SiTirelated antisite pair. As a consequence, the migrations of V_{Si}, , and Ti_{Si} have the close relationships to the recovery of radiation damages. Since Ti_{Si} locates in the Si atomic plane, it is expected that it can migrate via onlattice V_{Si} site along the Si atomic plane. The calculated migration energy barriers of V_{Si}, , and Ti_{Si} along the Si atomic plane are very low, only 0.9, 0.6, and 0.3 eV, respectively. This indicates that V_{Si}, , and Ti_{Si} defects can easily migrate along the region between the neighbouring nanotwined Ti_{3}C_{2} blocks. These processes provide quick recovery mechanisms for Ti_{3}SiC_{2} under radiation damage. The results also illustrate the predominant role of nanolaminated crystal structure on the excellent radiation tolerance of Ti_{3}SiC_{2}.
4. Conclusion
In summary, the stable defect structures, defect formation energies, and migration barriers of intrinsic point defects in Ti_{3}SiC_{2} are studied by using firstprinciples calculations. The results clearly show that the intercalated Si atomic plane, as well as the nanolaminated crystal structure of Ti_{3}SiC_{2}, not only provides new disorder mechanisms with low formation energies but also presents the quick migration paths of the related point defects. The reported disorder mechanisms with low formation energies are the antisite pair, Si Frenkel pair, and C Frenkel pair. The migration energy barriers of V_{Si}, , and Ti_{Si} along the Si atomic plane are only 0.9, 0.6, and 0.3 eV, respectively. The low formation energies of the defect pairs ensure the high ability of Ti_{3}SiC_{2} to accommodate structure disorders under displacive radiation damage. At the same time, the low migration energy barriers of point defects in Ti_{3}SiC_{2} indicate easy recovery of radiation damage. These theoretical results are helpful to explain the good radiation damage tolerance of Ti_{3}SiC_{2} and can shed a light on the theoretical predication of ceramics with good radiation damage tolerance. This further highlights a novel method to improve the radiation damage tolerance by developing nanoscalelayered structure which can serve as the sink or rapid recovery channel for radiationinduced point defects.
Conflict of Interests
The authors declare no conflict of interests.
Acknowledgments
Haibin Zhang is grateful to the foundation by the Recruitment Program of Global Youth Experts and the Youth Hundred Talents Project of Sichuan Province. This work was also supported by the Natural Sciences Foundation of China under Grant Nos. 50832008, 51372252, and 91326102, the Science and Technology Development Foundation of China Academy of Engineering Physics (Grants nos. 2012B0302035 and 2013A0301012), and Science and Technology Innovation Research Foundation of Institute of Nuclear Physics and Chemistry.
References
 M. W. Barsoum, “${\text{M}}_{N+1}{\text{A}\text{X}}_{N}$ phases: a new class of solids; thermodynamically stable nanolaminates,” Progress in Solid State Chemistry, vol. 28, no. 1–4, pp. 201–281, 2000. View at: Publisher Site  Google Scholar
 H. B. Zhang, Y. W. Bao, and Y. C. Zhou, “Current status in layered ternary carbide Ti_{3}SiC_{2}, a review,” Journal of Materials Science and Technology, vol. 25, no. 1, pp. 1–38, 2009. View at: Google Scholar
 Y. W. Bao, Y. C. Zhou, and H. B. Zhang, “Investigation on reliability of nanolayergrained Ti_{3}SiC_{2} via Weibull statistics,” Journal of Materials Science, vol. 42, no. 12, pp. 4470–4475, 2007. View at: Publisher Site  Google Scholar
 J. C. Nappé, P. Grosseau, F. Audubert et al., “Damages induced by heavy ions in titanium silicon carbide: effects of nuclear and electronic interactions at room temperature,” Journal of Nuclear Materials, vol. 385, no. 2, pp. 304–307, 2009. View at: Publisher Site  Google Scholar
 M. Le Flem, X. Liu, S. Doriot, T. Cozzika, and I. Monnet, “Irradiation damage in Ti_{3}(Si,Al)C_{2}: a TEM investigation,” International Journal of Applied Ceramic Technology, vol. 7, no. 6, pp. 766–775, 2010. View at: Publisher Site  Google Scholar
 K. R. Whittle, M. G. Blackford, R. D. Aughterson et al., “Radiation tolerance of ${\text{M}}_{n+1}{\text{A}\text{X}}_{n}$ phases, Ti_{3}AlC_{2} and Ti_{3}SiC_{2},” Acta Materialia, vol. 58, no. 13, pp. 4362–4368, 2010. View at: Publisher Site  Google Scholar
 J. C. Nappé, C. Maurice, P. Grosseau et al., “Microstructural changes induced by low energy heavy ion irradiation in titanium silicon carbide,” Journal of the European Ceramic Society, vol. 31, no. 8, pp. 1503–1511, 2011. View at: Publisher Site  Google Scholar
 X. M. Liu, M. Le Flem, J. Béchade, F. Onimus, T. Cozzika, and I. Monnet, “XRD investigation of ion irradiated Ti_{3}Si_{0.90}Al_{0.10}C_{2},” Nuclear Instruments and Methods in Physics Research B, vol. 268, no. 5, pp. 506–512, 2010. View at: Publisher Site  Google Scholar
 X. M. Liu, M. Le Flem, J. L. Béchade, and I. Monnet, “Nanoindentation investigation of heavy ion irradiated Ti_{3}(Si,Al)C_{2},” Journal of Nuclear Materials, vol. 401, no. 1–3, pp. 149–153, 2011. View at: Publisher Site  Google Scholar
 G. Kresse and J. Furthmüller, “Efficient iterative schemes for ab initio totalenergy calculations using a planewave basis set,” Physical Review B, vol. 54, no. 16, pp. 11169–11186, 1996. View at: Publisher Site  Google Scholar
 G. Kresse and J. Joubert, “From ultrasoft pseudopotentials to the projector augmentedwave method,” Physical Review B, vol. 59, no. 3, pp. 1758–1775, 1999. View at: Publisher Site  Google Scholar
 J. P. Perdew, K. Burke, and M. Ernzerhof, “Generalized gradient approximation made simple,” Physical Review Letters, vol. 77, no. 18, pp. 3865–3868, 1996. View at: Google Scholar
 J. D. Pack and H. J. Monkhorst, “‘Special points for Brillouinzone integrations’—a reply,” Physical Review B, vol. 16, no. 4, pp. 1748–1749, 1977. View at: Publisher Site  Google Scholar
 J. Y. Wang, Y. C. Zhou, T. Liao, J. Zhang, and Z. J. Lin, “A firstprinciples investigation of the phase stability of Ti_{2}AlC with Al vacancies,” Scripta Materialia, vol. 58, no. 3, pp. 227–230, 2008. View at: Publisher Site  Google Scholar
 T. Liao, J. Y. Wang, and Y. C. Zhou, “Ab initio modeling of the formation and migration of monovacancies in Ti_{2}AlC,” Scripta Materialia, vol. 59, no. 8, pp. 854–857, 2008. View at: Publisher Site  Google Scholar
 T. Liao, J. Y. Wang, and Y. C. Zhou, “Firstprinciples investigation of intrinsic defects and (N, O) impurity atom stimulated Al vacancy in Ti_{2}AlC,” Applied Physics Letters, vol. 93, no. 26, Article ID 261911, 3 pages, 2008. View at: Publisher Site  Google Scholar
 M. D. Segall, P. J. D. Lindan, M. J. Probert et al., “Firstprinciples simulation: ideas, illustrations and the CASTEP code,” Journal of Physics: Condensed Matter, vol. 14, no. 11, pp. 2717–2743, 2002. View at: Publisher Site  Google Scholar
 N. Govind, M. Petersen, G. Fitzgerald, D. KingSmith, and J. Andzelm, “A generalized synchronous transit method for transition state location,” Computational Materials Science, vol. 28, no. 2, pp. 250–258, 2003. View at: Publisher Site  Google Scholar
 L. Tsetseris and S. T. Pantelides, “Vacancies, interstitials and their complexes in titanium carbide,” Acta Materialia, vol. 56, no. 12, pp. 2864–2871, 2008. View at: Publisher Site  Google Scholar
 S. Kim, I. Szlufarska, and D. Morgan, “Ab initio study of point defect structures and energetics in ZrC,” Journal of Applied Physics, vol. 107, no. 5, Article ID 053521, 8 pages, 2010. View at: Publisher Site  Google Scholar
 K. E. Sickafus, L. Minervini, R. W. Grimes et al., “Radiation tolerance of complex oxides,” Science, vol. 289, no. 5480, pp. 748–751, 2000. View at: Publisher Site  Google Scholar
 G. Lucas and L. Pizzagalli, “Structure and stability of irradiationinduced Frenkel pairs in 3CSiC using first principles calculations,” Nuclear Instruments and Methods in Physics Research B, vol. 255, no. 1, pp. 124–129, 2007. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2013 Haibin Zhang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.